#------------------------------------------------------------------------------
#$Date: 2016-03-21 17:09:55 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178771 $
#$URL: svn://www.crystallography.net/cod/cif/4/10/25/4102594.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4102594
loop_
_publ_author_name
'Peng Wang'
'Scott Forbes'
'Taras Kolodiazhnyi'
'Kosuke Kosuda'
'Yurij Mozharivskyj'
_publ_section_title
;
 Synthesis, Crystal and Electronic Structures of New Narrow-Band-Gap
 Semiconducting Antimonide Oxides RE3SbO3 and RE8Sb3-\dO8, with RE = La,
 Sm, Gd, and Ho
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              8795
_journal_page_last               8803
_journal_paper_doi               10.1021/ja1027698
_journal_volume                  132
_journal_year                    2010
_chemical_formula_sum            'Ho8 O8 Sb3'
_chemical_formula_weight         1812.69
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.025(5)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   13.1445(17)
_cell_length_b                   3.7597(5)
_cell_length_c                   14.874(2)
_cell_measurement_temperature    296(2)
_cell_volume                     702.85(16)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.977
_diffrn_measured_fraction_theta_max 0.977
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0445
_diffrn_reflns_av_sigmaI/netI    0.0452
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       29
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_number            11917
_diffrn_reflns_theta_full        45.08
_diffrn_reflns_theta_max         45.08
_diffrn_reflns_theta_min         2.86
_exptl_absorpt_coefficient_mu    50.115
_exptl_crystal_density_diffrn    8.565
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1506
_refine_diff_density_max         5.669
_refine_diff_density_min         -6.458
_refine_diff_density_rms         0.823
_refine_ls_extinction_coef       0.00073(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.040
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     63
_refine_ls_number_reflns         3143
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.040
_refine_ls_R_factor_all          0.0467
_refine_ls_R_factor_gt           0.0353
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0227P)²+18.4291P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0666
_refine_ls_wR_factor_ref         0.0706
_reflns_number_gt                2633
_reflns_number_total             3143
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja1027698_si_009.cif
_cod_data_source_block           c2m
_cod_original_cell_volume        702.87(16)
_cod_database_code               4102594
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ho1 Ho 0.71909(2) 0.0000 0.089064(19) 0.00385(5) Uani 1 2 d S
Ho2 Ho 0.45656(2) 0.0000 0.16947(2) 0.00700(6) Uani 1 2 d S
Ho3 Ho 0.87733(2) 0.0000 0.34747(2) 0.00408(5) Uani 1 2 d S
Ho4 Ho 0.64392(2) 0.0000 0.42967(2) 0.00499(5) Uani 1 2 d S
Sb1 Sb 0.17149(3) 0.0000 0.26621(3) 0.00909(8) Uani 1 2 d S
Sb2 Sb 0.0000 0.0516(3) 0.0000 0.0084(3) Uani 0.473(2) 2 d SP
O1 O 0.4708(4) 0.0000 0.3689(5) 0.0133(10) Uani 1 2 d S
O2 O 0.8833(4) 0.0000 0.2024(3) 0.0055(7) Uani 1 2 d S
O3 O 0.2966(4) 0.0000 0.0662(3) 0.0064(7) Uani 1 2 d S
O4 O 0.1663(4) 0.0000 0.5151(4) 0.0072(7) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ho Ho -0.2175 4.6783 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ho1 O3 116.5(2) 3 3_545
O3 Ho1 O3 75.58(14) 3 5_655
O3 Ho1 O3 75.58(14) 3_545 5_655
O3 Ho1 O2 74.88(13) 3 .
O3 Ho1 O2 74.88(13) 3_545 .
O3 Ho1 O2 122.06(17) 5_655 .
O3 Ho1 Sb2 140.17(12) 3 3_545
O3 Ho1 Sb2 83.67(11) 3_545 3_545
O3 Ho1 Sb2 77.27(10) 5_655 3_545
O2 Ho1 Sb2 144.91(5) . 3_545
O3 Ho1 Sb2 83.67(11) 3 7
O3 Ho1 Sb2 140.17(12) 3_545 7
O3 Ho1 Sb2 77.27(10) 5_655 7
O2 Ho1 Sb2 144.91(5) . 7
Sb2 Ho1 Sb2 62.18(4) 3_545 7
O3 Ho1 Sb1 81.27(12) 3 3
O3 Ho1 Sb1 141.03(13) 3_545 3
O3 Ho1 Sb1 143.22(5) 5_655 3
O2 Ho1 Sb1 77.41(10) . 3
Sb2 Ho1 Sb1 104.853(15) 3_545 3
Sb2 Ho1 Sb1 72.058(14) 7 3
O3 Ho1 Sb1 141.03(13) 3 3_545
O3 Ho1 Sb1 81.27(12) 3_545 3_545
O3 Ho1 Sb1 143.22(5) 5_655 3_545
O2 Ho1 Sb1 77.41(10) . 3_545
Sb2 Ho1 Sb1 72.058(14) 3_545 3_545
Sb2 Ho1 Sb1 104.853(15) 7 3_545
Sb1 Ho1 Sb1 66.249(14) 3 3_545
O3 Ho1 Sb2 144.59(12) 3 7_545
O3 Ho1 Sb2 78.57(11) 3_545 7_545
O3 Ho1 Sb2 78.07(9) 5_655 7_545
O2 Ho1 Sb2 140.12(5) . 7_545
Sb2 Ho1 Sb2 5.48(4) 3_545 7_545
Sb2 Ho1 Sb2 67.663(11) 7 7_545
Sb1 Ho1 Sb2 107.538(14) 3 7_545
Sb1 Ho1 Sb2 69.522(13) 3_545 7_545
O3 Ho1 Sb2 78.57(11) 3 3
O3 Ho1 Sb2 144.59(12) 3_545 3
O3 Ho1 Sb2 78.07(9) 5_655 3
O2 Ho1 Sb2 140.12(5) . 3
Sb2 Ho1 Sb2 67.663(11) 3_545 3
Sb2 Ho1 Sb2 5.48(4) 7 3
Sb1 Ho1 Sb2 69.522(13) 3 3
Sb1 Ho1 Sb2 107.538(14) 3_545 3
Sb2 Ho1 Sb2 73.14(3) 7_545 3
O3 Ho1 Ho1 96.89(12) 3 7_645
O3 Ho1 Ho1 38.26(13) 3_545 7_645
O3 Ho1 Ho1 37.32(6) 5_655 7_645
O2 Ho1 Ho1 100.15(10) . 7_645
Sb2 Ho1 Ho1 77.883(14) 3_545 7_645
Sb2 Ho1 Ho1 109.865(16) 7 7_645
Sb1 Ho1 Ho1 177.237(14) 3 7_645
Sb1 Ho1 Ho1 114.654(11) 3_545 7_645
Sb2 Ho1 Ho1 75.155(13) 7_545 7_645
Sb2 Ho1 Ho1 112.211(15) 3 7_645
O3 Ho1 Ho1 38.26(13) 3 7_655
O3 Ho1 Ho1 96.89(12) 3_545 7_655
O3 Ho1 Ho1 37.32(6) 5_655 7_655
O2 Ho1 Ho1 100.15(10) . 7_655
Sb2 Ho1 Ho1 109.865(16) 3_545 7_655
Sb2 Ho1 Ho1 77.883(14) 7 7_655
Sb1 Ho1 Ho1 114.654(10) 3 7_655
Sb1 Ho1 Ho1 177.237(14) 3_545 7_655
Sb2 Ho1 Ho1 112.211(15) 7_545 7_655
Sb2 Ho1 Ho1 75.155(13) 3 7_655
Ho1 Ho1 Ho1 64.314(13) 7_645 7_655
O3 Ho2 O2 76.61(13) . 3_445
O3 Ho2 O2 76.61(13) . 3_455
O2 Ho2 O2 114.8(2) 3_445 3_455
O3 Ho2 O1 118.09(17) . .
O2 Ho2 O1 71.33(13) 3_445 .
O2 Ho2 O1 71.33(13) 3_455 .
O3 Ho2 Sb2 78.87(11) . 3_545
O2 Ho2 Sb2 85.29(11) 3_445 3_545
O2 Ho2 Sb2 143.14(12) 3_455 3_545
O1 Ho2 Sb2 145.38(4) . 3_545
O3 Ho2 Sb2 78.87(11) . 7
O2 Ho2 Sb2 143.14(12) 3_445 7
O2 Ho2 Sb2 85.29(11) 3_455 7
O1 Ho2 Sb2 145.38(4) . 7
Sb2 Ho2 Sb2 63.15(4) 3_545 7
O3 Ho2 Sb1 144.09(4) . 3
O2 Ho2 Sb1 137.99(12) 3_445 3
O2 Ho2 Sb1 78.28(11) 3_455 3
O1 Ho2 Sb1 76.59(9) . 3
Sb2 Ho2 Sb1 108.047(16) 3_545 3
Sb2 Ho2 Sb1 73.840(15) 7 3
O3 Ho2 Sb1 144.09(4) . 3_545
O2 Ho2 Sb1 78.28(11) 3_445 3_545
O2 Ho2 Sb1 137.99(12) 3_455 3_545
O1 Ho2 Sb1 76.59(9) . 3_545
Sb2 Ho2 Sb1 73.840(15) 3_545 3_545
Sb2 Ho2 Sb1 108.047(16) 7 3_545
Sb1 Ho2 Sb1 68.331(14) 3 3_545
O3 Ho2 Sb2 79.59(10) . 7_545
O2 Ho2 Sb2 80.10(11) 3_445 7_545
O2 Ho2 Sb2 147.59(12) 3_455 7_545
O1 Ho2 Sb2 140.40(4) . 7_545
Sb2 Ho2 Sb2 5.52(4) 3_545 7_545
Sb2 Ho2 Sb2 68.669(12) 7 7_545
Sb1 Ho2 Sb2 110.697(15) 3 7_545
Sb1 Ho2 Sb2 71.097(14) 3_545 7_545
O3 Ho2 Sb2 79.59(10) . 3
O2 Ho2 Sb2 147.59(12) 3_445 3
O2 Ho2 Sb2 80.10(11) 3_455 3
O1 Ho2 Sb2 140.40(4) . 3
Sb2 Ho2 Sb2 68.669(12) 3_545 3
Sb2 Ho2 Sb2 5.52(4) 7 3
Sb1 Ho2 Sb2 71.097(14) 3 3
Sb1 Ho2 Sb2 110.697(15) 3_545 3
Sb2 Ho2 Sb2 74.19(4) 7_545 3
O3 Ho2 Ho1 36.85(6) . 3_445
O2 Ho2 Ho1 39.81(12) 3_445 3_445
O2 Ho2 Ho1 97.29(11) 3_455 3_445
O1 Ho2 Ho1 97.55(9) . 3_445
Sb2 Ho2 Ho1 78.363(13) 3_545 3_445
Sb2 Ho2 Ho1 110.771(14) 7 3_445
Sb1 Ho2 Ho1 173.498(14) 3 3_445
Sb1 Ho2 Ho1 113.384(11) 3_545 3_445
Sb2 Ho2 Ho1 75.593(12) 7_545 3_445
Sb2 Ho2 Ho1 113.079(13) 3 3_445
O3 Ho2 Ho1 36.85(6) . 3_455
O2 Ho2 Ho1 97.29(11) 3_445 3_455
O2 Ho2 Ho1 39.81(12) 3_455 3_455
O1 Ho2 Ho1 97.55(9) . 3_455
Sb2 Ho2 Ho1 110.771(14) 3_545 3_455
Sb2 Ho2 Ho1 78.363(13) 7 3_455
Sb1 Ho2 Ho1 113.384(11) 3 3_455
Sb1 Ho2 Ho1 173.498(14) 3_545 3_455
Sb2 Ho2 Ho1 113.079(13) 7_545 3_455
Sb2 Ho2 Ho1 75.593(12) 3 3_455
Ho1 Ho2 Ho1 64.180(12) 3_445 3_455
O2 Ho3 O1 87.91(19) . 3
O2 Ho3 O1 87.91(18) . 3_545
O1 Ho3 O1 116.0(2) 3 3_545
O2 Ho3 O4 168.05(17) . 5_656
O1 Ho3 O4 98.35(18) 3 5_656
O1 Ho3 O4 98.35(18) 3_545 5_656
O2 Ho3 Sb1 84.17(10) . 3_545
O1 Ho3 Sb1 156.48(13) 3 3_545
O1 Ho3 Sb1 85.90(12) 3_545 3_545
O4 Ho3 Sb1 86.13(10) 5_656 3_545
O2 Ho3 Sb1 84.17(10) . 3
O1 Ho3 Sb1 85.90(12) 3 3
O1 Ho3 Sb1 156.48(13) 3_545 3
O4 Ho3 Sb1 86.13(10) 5_656 3
Sb1 Ho3 Sb1 71.311(14) 3_545 3
O2 Ho3 Ho4 127.83(12) . .
O1 Ho3 Ho4 116.11(14) 3 .
O1 Ho3 Ho4 116.11(14) 3_545 .
O4 Ho3 Ho4 40.22(12) 5_656 .
Sb1 Ho3 Ho4 54.941(11) 3_545 .
Sb1 Ho3 Ho4 54.941(11) 3 .
O2 Ho3 Ho2 34.89(5) . 3_545
O1 Ho3 Ho2 106.15(16) 3 3_545
O1 Ho3 Ho2 53.28(17) 3_545 3_545
O4 Ho3 Ho2 148.576(18) 5_656 3_545
Sb1 Ho3 Ho2 79.258(12) 3_545 3_545
Sb1 Ho3 Ho2 114.572(14) 3 3_545
Ho4 Ho3 Ho2 134.197(9) . 3_545
O2 Ho3 Ho2 34.89(5) . 3
O1 Ho3 Ho2 53.28(17) 3 3
O1 Ho3 Ho2 106.15(16) 3_545 3
O4 Ho3 Ho2 148.576(18) 5_656 3
Sb1 Ho3 Ho2 114.572(14) 3_545 3
Sb1 Ho3 Ho2 79.258(12) 3 3
Ho4 Ho3 Ho2 134.197(8) . 3
Ho2 Ho3 Ho2 62.204(11) 3_545 3
O2 Ho3 Ho3 90.0 . 1_565
O1 Ho3 Ho3 32.02(12) 3 1_565
O1 Ho3 Ho3 147.98(12) 3_545 1_565
O4 Ho3 Ho3 90.0 5_656 1_565
Sb1 Ho3 Ho3 125.655(7) 3_545 1_565
Sb1 Ho3 Ho3 54.345(7) 3 1_565
Ho4 Ho3 Ho3 90.0 . 1_565
Ho2 Ho3 Ho3 121.102(6) 3_545 1_565
Ho2 Ho3 Ho3 58.898(6) 3 1_565
O2 Ho3 Ho3 90.0 . 1_545
O1 Ho3 Ho3 147.98(12) 3 1_545
O1 Ho3 Ho3 32.02(12) 3_545 1_545
O4 Ho3 Ho3 90.0 5_656 1_545
Sb1 Ho3 Ho3 54.345(7) 3_545 1_545
Sb1 Ho3 Ho3 125.655(7) 3 1_545
Ho4 Ho3 Ho3 90.0 . 1_545
Ho2 Ho3 Ho3 58.898(6) 3_545 1_545
Ho2 Ho3 Ho3 121.102(6) 3 1_545
Ho3 Ho3 Ho3 180.000(17) 1_565 1_545
O2 Ho3 Ho1 33.54(12) . .
O1 Ho3 Ho1 105.18(16) 3 .
O1 Ho3 Ho1 105.18(16) 3_545 .
O4 Ho3 Ho1 134.51(12) 5_656 .
Sb1 Ho3 Ho1 57.982(10) 3_545 .
Sb1 Ho3 Ho1 57.982(10) 3 .
Ho4 Ho3 Ho1 94.283(13) . .
Ho2 Ho3 Ho1 56.781(10) 3_545 .
Ho2 Ho3 Ho1 56.781(10) 3 .
Ho3 Ho3 Ho1 90.0 1_565 .
Ho3 Ho3 Ho1 90.0 1_545 .
O1 Ho4 O4 100.48(15) . 3
O1 Ho4 O4 100.48(15) . 3_545
O4 Ho4 O4 114.2(2) 3 3_545
O1 Ho4 O4 176.0(2) . 5_656
O4 Ho4 O4 81.64(14) 3 5_656
O4 Ho4 O4 81.64(14) 3_545 5_656
O1 Ho4 Sb1 91.25(14) . 3_545
O4 Ho4 Sb1 154.89(12) 3 3_545
O4 Ho4 Sb1 84.96(11) 3_545 3_545
O4 Ho4 Sb1 85.50(10) 5_656 3_545
O1 Ho4 Sb1 91.25(14) . 3
O4 Ho4 Sb1 84.96(11) 3 3
O4 Ho4 Sb1 154.89(12) 3_545 3
O4 Ho4 Sb1 85.50(10) 5_656 3
Sb1 Ho4 Sb1 72.559(15) 3_545 3
O1 Ho4 Ho4 142.77(8) . 7_656
O4 Ho4 Ho4 42.40(12) 3 7_656
O4 Ho4 Ho4 99.35(12) 3_545 7_656
O4 Ho4 Ho4 39.24(6) 5_656 7_656
Sb1 Ho4 Ho4 121.696(16) 3_545 7_656
Sb1 Ho4 Ho4 83.703(13) 3 7_656
O1 Ho4 Ho4 142.77(8) . 7_646
O4 Ho4 Ho4 99.35(12) 3 7_646
O4 Ho4 Ho4 42.40(12) 3_545 7_646
O4 Ho4 Ho4 39.24(6) 5_656 7_646
Sb1 Ho4 Ho4 83.703(13) 3_545 7_646
Sb1 Ho4 Ho4 121.696(16) 3 7_646
Ho4 Ho4 Ho4 64.911(13) 7_656 7_646
O1 Ho4 Ho3 137.91(18) . .
O4 Ho4 Ho3 102.02(12) 3 .
O4 Ho4 Ho3 102.02(12) 3_545 .
O4 Ho4 Ho3 38.06(12) 5_656 .
Sb1 Ho4 Ho3 56.196(10) 3_545 .
Sb1 Ho4 Ho3 56.196(10) 3 .
Ho4 Ho4 Ho3 66.204(12) 7_656 .
Ho4 Ho4 Ho3 66.204(12) 7_646 .
O1 Ho4 O1 73.5(2) . 5_656
O4 Ho4 O1 63.94(12) 3 5_656
O4 Ho4 O1 63.94(12) 3_545 5_656
O4 Ho4 O1 110.57(15) 5_656 5_656
Sb1 Ho4 O1 141.14(3) 3_545 5_656
Sb1 Ho4 O1 141.14(3) 3 5_656
Ho4 Ho4 O1 87.63(7) 7_656 5_656
Ho4 Ho4 O1 87.63(7) 7_646 5_656
Ho3 Ho4 O1 148.62(9) . 5_656
O1 Ho4 Ho4 90.000(1) . 1_565
O4 Ho4 Ho4 32.92(11) 3 1_565
O4 Ho4 Ho4 147.08(11) 3_545 1_565
O4 Ho4 Ho4 90.0 5_656 1_565
Sb1 Ho4 Ho4 126.280(8) 3_545 1_565
Sb1 Ho4 Ho4 53.720(8) 3 1_565
Ho4 Ho4 Ho4 57.545(7) 7_656 1_565
Ho4 Ho4 Ho4 122.455(7) 7_646 1_565
Ho3 Ho4 Ho4 90.0 . 1_565
O1 Ho4 Ho4 90.0 5_656 1_565
O1 Ho4 Ho4 90.000(1) . 1_545
O4 Ho4 Ho4 147.08(11) 3 1_545
O4 Ho4 Ho4 32.92(11) 3_545 1_545
O4 Ho4 Ho4 90.0 5_656 1_545
Sb1 Ho4 Ho4 53.720(8) 3_545 1_545
Sb1 Ho4 Ho4 126.280(8) 3 1_545
Ho4 Ho4 Ho4 122.455(7) 7_656 1_545
Ho4 Ho4 Ho4 57.545(7) 7_646 1_545
Ho3 Ho4 Ho4 90.0 . 1_545
O1 Ho4 Ho4 90.0 5_656 1_545
Ho4 Ho4 Ho4 180.0 1_565 1_545
Ho4 Sb1 Ho4 72.559(15) 3_455 3_445
Ho4 Sb1 Ho3 68.863(11) 3_455 3_455
Ho4 Sb1 Ho3 109.223(16) 3_445 3_455
Ho4 Sb1 Ho3 109.223(16) 3_455 3_445
Ho4 Sb1 Ho3 68.863(11) 3_445 3_445
Ho3 Sb1 Ho3 71.311(14) 3_455 3_445
Ho4 Sb1 Ho2 112.971(16) 3_455 3_445
Ho4 Sb1 Ho2 74.078(12) 3_445 3_445
Ho3 Sb1 Ho2 176.683(16) 3_455 3_445
Ho3 Sb1 Ho2 110.098(11) 3_445 3_445
Ho4 Sb1 Ho2 74.078(12) 3_455 3_455
Ho4 Sb1 Ho2 112.971(16) 3_445 3_455
Ho3 Sb1 Ho2 110.098(11) 3_455 3_455
Ho3 Sb1 Ho2 176.683(16) 3_445 3_455
Ho2 Sb1 Ho2 68.331(14) 3_445 3_455
Ho4 Sb1 Ho1 175.317(13) 3_455 3_445
Ho4 Sb1 Ho1 110.484(11) 3_445 3_445
Ho3 Sb1 Ho1 106.548(15) 3_455 3_445
Ho3 Sb1 Ho1 69.375(11) 3_445 3_445
Ho2 Sb1 Ho1 71.564(12) 3_445 3_445
Ho2 Sb1 Ho1 107.309(16) 3_455 3_445
Ho4 Sb1 Ho1 110.484(11) 3_455 3_455
Ho4 Sb1 Ho1 175.317(13) 3_445 3_455
Ho3 Sb1 Ho1 69.375(11) 3_455 3_455
Ho3 Sb1 Ho1 106.548(15) 3_445 3_455
Ho2 Sb1 Ho1 107.309(16) 3_445 3_455
Ho2 Sb1 Ho1 71.564(12) 3_455 3_455
Ho1 Sb1 Ho1 66.249(14) 3_445 3_455
Ho2 Sb2 Ho2 116.85(4) 3_455 7
Ho2 Sb2 Ho1 75.49(2) 3_455 3_455
Ho2 Sb2 Ho1 73.12(2) 7 3_455
Ho2 Sb2 Ho1 73.12(2) 3_455 7
Ho2 Sb2 Ho1 75.49(2) 7 7
Ho1 Sb2 Ho1 117.82(4) 3_455 7
Ho2 Sb2 Ho2 174.48(4) 3_455 7_545
Ho2 Sb2 Ho2 68.669(12) 7 7_545
Ho1 Sb2 Ho2 107.028(10) 3_455 7_545
Ho1 Sb2 Ho2 109.273(10) 7 7_545
Ho2 Sb2 Ho2 68.669(12) 3_455 3_445
Ho2 Sb2 Ho2 174.48(4) 7 3_445
Ho1 Sb2 Ho2 109.273(10) 3_455 3_445
Ho1 Sb2 Ho2 107.028(10) 7 3_445
Ho2 Sb2 Ho2 105.81(4) 7_545 3_445
Ho2 Sb2 Ho1 107.058(10) 3_455 7_545
Ho2 Sb2 Ho1 109.307(10) 7 7_545
Ho1 Sb2 Ho1 174.52(4) 3_455 7_545
Ho1 Sb2 Ho1 67.663(11) 7 7_545
Ho2 Sb2 Ho1 70.01(2) 7_545 7_545
Ho2 Sb2 Ho1 67.865(19) 3_445 7_545
Ho2 Sb2 Ho1 109.307(10) 3_455 3_445
Ho2 Sb2 Ho1 107.058(10) 7 3_445
Ho1 Sb2 Ho1 67.663(11) 3_455 3_445
Ho1 Sb2 Ho1 174.52(4) 7 3_445
Ho2 Sb2 Ho1 67.865(19) 7_545 3_445
Ho2 Sb2 Ho1 70.01(2) 3_445 3_445
Ho1 Sb2 Ho1 106.86(3) 7_545 3_445
Ho4 O1 Ho3 121.65(12) . 3_445
Ho4 O1 Ho3 121.65(12) . 3_455
Ho3 O1 Ho3 116.0(2) 3_445 3_455
Ho4 O1 Ho2 99.7(2) . .
Ho3 O1 Ho2 89.19(18) 3_445 .
Ho3 O1 Ho2 89.19(18) 3_455 .
Ho4 O1 Ho4 106.5(2) . 5_656
Ho3 O1 Ho4 77.18(16) 3_445 5_656
Ho3 O1 Ho4 77.18(16) 3_455 5_656
Ho2 O1 Ho4 153.73(18) . 5_656
Ho3 O2 Ho2 111.10(13) . 3
Ho3 O2 Ho2 111.10(13) . 3_545
Ho2 O2 Ho2 114.8(2) 3 3_545
Ho3 O2 Ho1 115.1(2) . .
Ho2 O2 Ho1 102.13(14) 3 .
Ho2 O2 Ho1 102.13(14) 3_545 .
Ho1 O3 Ho1 116.5(2) 3_445 3_455
Ho1 O3 Ho2 106.29(14) 3_445 .
Ho1 O3 Ho2 106.29(14) 3_455 .
Ho1 O3 Ho1 104.42(14) 3_445 5_655
Ho1 O3 Ho1 104.42(14) 3_455 5_655
Ho2 O3 Ho1 119.6(2) . 5_655
Ho4 O4 Ho4 114.2(2) 3_445 3_455
Ho4 O4 Ho3 118.90(12) 3_445 5_656
Ho4 O4 Ho3 118.90(12) 3_455 5_656
Ho4 O4 Ho4 98.36(14) 3_445 5_656
Ho4 O4 Ho4 98.36(14) 3_455 5_656
Ho3 O4 Ho4 101.72(19) 5_656 5_656
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ho1 O3 2.211(3) 3
Ho1 O3 2.211(3) 3_545
Ho1 O3 2.258(5) 5_655
Ho1 O2 2.317(5) .
Ho1 Sb2 3.2645(8) 3_545
Ho1 Sb2 3.2644(8) 7
Ho1 Sb1 3.4400(6) 3
Ho1 Sb1 3.4400(6) 3_545
Ho1 Sb2 3.4807(8) 7_545
Ho1 Sb2 3.4807(8) 3
Ho1 Ho1 3.5319(6) 7_645
Ho1 Ho1 3.5319(6) 7_655
Ho2 O3 2.211(5) .
Ho2 O2 2.231(3) 3_445
Ho2 O2 2.231(3) 3_455
Ho2 O1 2.917(7) .
Ho2 Sb2 3.2195(8) 3_545
Ho2 Sb2 3.2195(8) 7
Ho2 Sb1 3.3474(5) 3
Ho2 Sb1 3.3474(5) 3_545
Ho2 Sb2 3.4386(9) 7_545
Ho2 Sb2 3.4386(9) 3
Ho2 Ho1 3.5386(5) 3_445
Ho2 Ho1 3.5385(5) 3_455
Ho3 O2 2.182(5) .
Ho3 O1 2.217(3) 3
Ho3 O1 2.217(3) 3_545
Ho3 O4 2.279(5) 5_656
Ho3 Sb1 3.2250(5) 3_545
Ho3 Sb1 3.2250(5) 3
Ho3 Ho4 3.6199(6) .
Ho3 Ho2 3.6391(5) 3_545
Ho3 Ho2 3.6391(5) 3
Ho3 Ho3 3.7597(5) 1_565
Ho3 Ho3 3.7597(5) 1_545
Ho4 O1 2.189(5) .
Ho4 O4 2.240(3) 3
Ho4 O4 2.240(3) 3_545
Ho4 O4 2.387(5) 5_656
Ho4 Sb1 3.1769(5) 3_545
Ho4 Sb1 3.1769(5) 3
Ho4 Ho4 3.5030(6) 7_656
Ho4 Ho4 3.5030(6) 7_646
Ho4 O1 3.728(7) 5_656
Ho4 Ho4 3.7597(5) 1_565
Ho4 Ho4 3.7597(5) 1_545
Sb1 Ho4 3.1769(5) 3_455
Sb1 Ho4 3.1769(5) 3_445
Sb1 Ho3 3.2250(5) 3_455
Sb1 Ho3 3.2250(5) 3_445
Sb1 Ho2 3.3474(5) 3_445
Sb1 Ho2 3.3474(5) 3_455
Sb1 Ho1 3.4400(5) 3_445
Sb1 Ho1 3.4400(5) 3_455
Sb2 Ho2 3.2195(8) 3_455
Sb2 Ho2 3.2195(8) 7
Sb2 Ho1 3.2645(8) 3_455
Sb2 Ho1 3.2644(8) 7
Sb2 Ho2 3.4386(9) 7_545
Sb2 Ho2 3.4386(9) 3_445
Sb2 Ho1 3.4807(8) 7_545
Sb2 Ho1 3.4807(8) 3_445
O1 Ho3 2.217(3) 3_445
O1 Ho3 2.217(3) 3_455
O1 Ho4 3.728(7) 5_656
O2 Ho2 2.231(3) 3
O2 Ho2 2.231(3) 3_545
O3 Ho1 2.211(3) 3_445
O3 Ho1 2.211(3) 3_455
O3 Ho1 2.258(5) 5_655
O4 Ho4 2.240(3) 3_445
O4 Ho4 2.240(3) 3_455
O4 Ho3 2.279(5) 5_656
O4 Ho4 2.387(5) 5_656
